Structure of Silica Gel Si-60 and Pyrocarbon/Silica Gel Adsorbents Thermally and Hydrothermally
Embed Size (px)
Transcript of Structure of Silica Gel Si-60 and Pyrocarbon/Silica Gel Adsorbents Thermally and Hydrothermally
Structure of Silica Gel Si-60 and Pyrocarbon/Silica GelAdsorbents Thermally and Hydrothermally Treated
V. M. Gun’ko,*,† R. Leboda,‡ J. Skubiszewska-Zieba,‡ V. V. Turov,† andP. Kowalczyk§
Institute of Surface Chemistry, 17 General Naumov Street, 03164 Kiev, Ukraine, Departmentof Chemical Physics, Maria Curie-Sklodowska University, 20-031 Lublin, Poland, and
Military Institute of Chemistry and Radiometry, 00-910 Warsaw, Poland
Received July 31, 2000. In Final Form: November 30, 2000
Characteristics of porous structure of silica gel Si-60 (pristine and covered by different amounts ofpyrocarbon prepared by pyrolysis of acenaphthene, acetylacetone, and glucose, then heated at 500 °C inair or hydrothermally treated (HTT) at 150 or 200 °C, and also heated at 500 °C) were analyzed by usingTEM, 1H NMR, and adsorption-desorption of nitrogen at 77.35 K. The structural parameters were estimatedby the direct minimization method or the overall isotherm approximation with a regularization procedure.Pyrolysis of different organics on Si-60 is accompanied by marked changes in the pore structure dependingon the nature of precursors. Hydrothermal treatment of silica gel and carbosils at 150-200 °C for 6 hresults in a strong modification of both pores and outer surfaces of silica gel particles in contrast to heatingof pristine Si-60 or carbosils (after HTT) at 500 °C in air for 24 h. Computations of the distributions ofthe pore size and nitrogen adsorption energy, as well as 1H NMR spectra of the interfacial water, revealan increase in the adsorbent nonuniformity due to hydrothermal treatment, but heating of silica gel andpyrocarbon/silica in air gives the opposite result.
IntroductionPyrocarbon/silicas (carbosils) can be appropriate as
adsorbents utilized in different media due to their abilityto interact effectively with polar and nonpolar com-pounds.1,2 The characteristics of carbon deposits andadsorbent as a whole can be changed due to variations inpyrolysis conditions, precursor origin, or pretreatmenttechniques (chemical modification, hydrothermal andthermal treatments).1-6 It is known4-8 that both thermaland hydrothermal treatments (HTT) of silica gels changethe pore structure, namely, decrease the specific surfacearea and increase average pore size, depending on thetreatment temperature. One can assume that markedstructural alterations in the silica matrix can occur duringpyrolysis of organics at 500-700 °C, depending on thenature of reactants. It should be noted that the influenceof hydrothermal treatment of hybrid carbon/mineraladsorbents on their texture is inadequately investigated,as well as the impact of the origin of carbonized precursorson the structural parameters of hybrid adsorbents dif-ferently treated. Therefore, the aim of this work is to studythe impact of pyrolysis of different precursors (acenaph-
thene, acetylacetone, glucose) on the silica gel (Si-60)surfaces and thermal and hydrothermal treatments ofcarbosils on their structural characteristics in comparisonwith those for initial, heated, or hydrothermally treatedsilica gels.
(a) Materials. Silica gel Si-60 (Merck) was used as the initialmaterial (grain fraction of 0.1-0.2 mm) to prepare pyrocarbon/silica adsorbents (carbosils) with different concentrations ofpyrocarbon (CC). For comparison, silica gels Si-40 (Merck) (specificsurface area SBET ) 732 m2/g, total pore volume Vp ) 0.542 cm3/g, average pore radius Rp ) 1.48 nm), Si-40-HTT (THTT ) 150 °C,SBET ) 309 m2/g, Vp ) 0.512 cm3/g, Rp ) 3.31 nm; or THTT ) 200°C, SBET ) 107 m2/g, Vp ) 0.497 cm3/g, Rp ) 9.3 nm); Si-100(Merck) (SBET ) 332 m2/g, Vp ) 1.153 cm3/g, Rp ) 6.95 nm), andSi-100-HTT (THTT ) 200 °C, SBET ) 49 m2/g, Vp ) 0.18 cm3/g, Rp) 7.7 nm) were utilized. Silica gel was dried at 200 °C for 24 hthen cooled in a desiccator before the pyrolysis of depositedacenaphthene (0.5, 2, or 3 g per 5 g of Si-60 corresponding toAN1, AN2, and AN3 samples at CC ) 7.0, 15.8, and 22.7 wt %,respectively) in a stainless steel autoclave (0.3 L) at 500 °C for6 h. The pyrolysis of acetylacetone adsorbed in the amounts of0.02, 0.03, and 0.04 M per 5 g of Si-60 gave the series of carbosilsAC1, AC2, and AC3 (CC ) 4, 9.1, and 14.5 wt %, respectively).The carbonization of glucose (6 g per 10 g of Si-60) gave carbosilGL (CC ) 16.5 wt %). After the reaction, all the prepared carbosilswere washed in a Soxhlet apparatus with N,N-dimethylforma-mide and acetone. Then after removal of substances not boundto the solid surfaces, the samples were dried at 200 °C.
Hydrothermal treatment of adsorbents (labeled HTT) wascarried out in the autoclave at 150 or 200 °C for 6 h. Sample (2g) of silica gel or carbosil was placed in a quartz vessel in theautoclave containing 20 mL of water, which was heated at 150°C (Si-60, Si-40, GL, ANi) or 200 °C (Si-60, Si-40, Si-100, ACi)(these conditions ensured saturated water vapor pressure in theautoclave9). After the modification, the samples were dried at200 °C for 6 h. To investigate the pyrolysis impact of differentprecursorsonthesilicamatrixstructure,pyrocarbonwasremovedon heating at 500 °C for 24 h in air (labeled T). The amounts of
* To whom correspondence should be addressed. Fax: 380 444443567. E-mail: [email protected].
† Institute of Surface Chemistry.‡ Maria Curie-Sklodowska University.§ Military Institute of Chemistry and Radiometry.(1) (a) Adsorption on New and Modified Inorganic Sorbents; Dab-
rowski, A., Tertykh, V. A., Eds.; Elsevier: Amsterdam, 1996. (b) Leboda,R. Mater. Chem. Phys. 1992, 31, 243; 1993, 34, 123.
(2) Leboda, R. Polish Appl. Chem. 1988, 32, 229.(3) McDaniel, M. P.; Hottovy, T. D. J. Colloid Interface Sci. 1980, 78,
31(4) Leboda, R.; Mendyk, E.; Gierak, A.; Tertykh, V. A. Colloid. Surf.
A 1995, 105, 181.(5) Leboda, R.; Mendyk, E.; Gierak, A.; Tertykh, V. A. Colloid. Surf.
A 1995, 105, 191.(6) Leboda, R.; Mendyk, E. Mater. Chem. Phys. 1991, 27, 189.(7) The Surface Properties of Silicas; Legrand, A. P., Ed.; Wiley: New
York, 1998.(8) Proc. Int. Conf. Silica Sci. Technol. “Silica 98”; Mulhouse: France,
Sept 1-4, 1998. (9) Physicochemical Hanbook; WNT: Warsaw, 1974; p 132.
3148 Langmuir 2001, 17, 3148-3161
10.1021/la001094t CCC: $20.00 © 2001 American Chemical SocietyPublished on Web 04/27/2001
carbon deposits CC were determined gravimetrically from thedifferences between weights of dry samples before and afterthermal treatment at 500 °C in air.
(b) Transmission Electron Microscopy. TEM micrographsof carbosil samples were made with a BS 540 (Tesla) apparatus(accelerating voltage 80 kV, resolution 0.8 nm, magnification×24 000). Microscope samples were prepared by the platinum-carbon replication method with evaporation of carbon andplatinum onto the adsorbent surface then treated in hydrofluoricacid to dissolve oxides.
(c) Nitrogen Adsorption-Desorption. The specific surfacearea SBET,10 pore volume Vp (estimated at p/p0 ≈ 0.98, where pand p0 denote the equilibrium and saturation pressures ofnitrogen, respectively), average pore radii Rp, and other poreparameters listed in Table 1 were determined from nitrogenadsorption-desorption at 77.35 K measured with a Sorptomat1900 (Carlo Erba, Milan) apparatus or a Micromeritics ASAP2010 adsorption analyzer. Additionally, the total pore volume VΣ
was evaluated using titration method3 with methanol as a titrantadded to weighted dry sample. The endpoint of titration wasreached when powdered adsorbent lost its free-flowing characterdue to wetness. Typically, VΣ is slightly larger than Vp (Table 1).
The micropore parameters (VDS, SDS) were estimated usingthe modified Dubinin-Stoeckli equation11
where xDS is the pore half-width; δ is the distribution dispersion
(δDS in Table 1); Z ) (1 + 2mδ2A2)0.5; m ) (âk)-2; erf(z) )(2/xπ)∫0
ze-t2 dt; n is the varied equation parameter; A ) RTln(p0/p) is the differential molar work equal, with inverse sign,to the variation in the Gibbs free energy; âN2 ) 0.33; and k ) 10kJ nm/mol. The micropore parameters were computed withoutcorrection on the adsorption in mesopores, as integration for SDSand VDS was performed at Rp < 1 nm (however, this approachcan result in some overestimation of the SDS and VDS values).The specific surface area of mesopores (Smes) was computed withthe theory of capillary condensation-evaporation with Broekhoff-deBoer-Dollimore-Heal-Dubinin-Ulin corrections to the Kelvinequation,12,13 which links the adsorbed layer thickness (t) andthe radius (Rp > 1 nm) of filled pores (empted on desorption),using the direct minimization method with the program packagedescribed in detail elsewhere.14
The Fowler-Guggenheim (FG) equation describing localizedmonolayer adsorption with lateral interaction10,15
(where K ) K0(T) exp(E/kBT) is the Langmuir constant, z is thenumber of nearest neighbors of an adsorbate molecule (assumingz ) 4), w is the interaction energy between a pair of nearestneighbors, kB is the Boltzmann constant, and zw/kB ) 380 K15
close to the liquefaction heat QL) was used as a kernel Θl in theoverall adsorption isotherm in the form of a Fredholm integral
(10) (a) Adamson, A. W.; Gast, A. P. Physical Chemistry of Surface,6th ed.; Wiley: New York, 1997. (b) Characterization of Porous Solids;Gregg, S. J., Sing, K. S. W., Stoeckli, H. F., Eds.; Soc. Chem. Industry:London, 1979. (c) Gregg, S. J.; Sing, K. S. W. Adsorption, Surface Areaand Porosity, 2nd ed.; Academic Press: London, 1982. (d) Fenelonov,V. B. Porous Carbon; Nauka: Novosibirsk, 1995.
(11) Dubinin, M. M.; Stoeckli, F. J. Colloid Interface Sci. 1980, 75,34.
(12) (a) Dollimore, D.; Heal, C. R. J. Appl. Chem. 1964, 14, 109. (b)Broekhoff, J. C.; deBoer, J. H. J. Catal. 1967, 9, 8; 1968, 10, 153.
(13) Dubinin, M. M.; Kataeva, L. I.; Ulin, B. I. Izv. AN USSR, Ser.Khim. 1977, No. 3, 510.
(14) (a) Gun’ko, V. M. Zh. Fiz. Khim. 1989, 63, 506. (b) Gun’ko, V.M.; Lukyanchuk, V. M.; Chuiko, A. A. Catal. Catal. 1992, No. 28, 82.(c) Gun’ko, V. M. Teoret. Eksperim. Khim. 2000, 36, 1.
(15) (a) Hill, T. L. Statistical Thermodynamics; McGraw-Hill: NewYork, 1956. (b) Choma, J.; Jaroniec, M. Langmuir 1997, 13, 1026. (c)Jaroniec, C. P.; Jaroniec, M.; Kruk, M. J. Chromatogr. A 1998, 797, 93.
Table 1. Structural Parameters of Initial and Modified Si-60, Thermally Treated (T) at 500 °C and HydrothermallyTreated (HTT) at 150 °C (Si-60, AN, GL) and 200 °C (Si-60, AC)
adsorbent CC, wt % SBET, m2/g Vp, cm3/g Rp, nm VΣ, cm3/g SR, m2/g Smes, m2/g SDS, m2/g VDS, cm3/g xDS, nm δDS, nm
Si-60 369 0.753 4.1 0.753 363 363 169 0.19 0.90 0.49Si-60-T 362 0.747 4.1 0.750 361 343 154 0.02 0.99 0.21Si-60-HTT-150 121 0.731 12.1 0.790 120 151 36 0.08 1.03 0.14Si-60-HTT-150-T 122 0.738 12.1 0.800 115 147 33 0.07 1.06 0.19Si-60-HTT-200 47 0.272 11.8 40 27 26 0.03 0.63 0.54Si-60-HTT-200-T 46 0.305 13.0 45 27 29 0.03 0.84 0.44AN1 7 327 0.650 4.8 0.662 309 290 159 0.18 0.94 0.39AN1-T 365 0.736 4.0 0.750 357 381 151 0.20 0.10 0.38AN1-HTT 189 0.613 6.5 0.674 181 201 106 0.13 0.86 0.66AN1-HTT-T 212 0.711 6.7 0.750 203 236 114 0.14 0.82 0.65AN2 15.8 244 0.480 3.9 0.557 244 312 108 0.13 0.96 0.40AN2-T 358 0.725 4.0 0.750 362 351 147 0.19 0.98 0.33AN2-HTT 167 0.478 5.7 0.560 150 132 59 0.09 0.88 0.89AN2-HTT-T 181 0.714 7.9 0.750 166 253 130 0.13 0.61 0.61AN3 22.7 233 0.453 3.9 0.448 222 306 116 0.15 0.98 0.52AN3-T 337 0.726 4.3 0.750 372 361 140 0.09 1.12 0.12AN3-HTT 150 0.385 5.1 0.450 148 117 79 0.11 0.99 0.59AN3-HTT-T 173 0.698 8.0 0.750 163 212 95 0.10 0.88 0.38AC1 4 339 0.717 4.2 0.700 327 328 159 0.18 0.93 0.41AC1-T 345 0.743 4.3 0.750 365 0.19 1.03AC1-HTT 68 0.634 19.5 0.735 64 63 13 0.03 1.11 0.23AC1-HTT-T 60 0.709 23.5 0.780 59 68 28 0.04 1.03 0.45AC2 9.1 296 0.606 4.1 0.670 287 290 154 0.18 0.94 0.44AC2-T 340 0.730 4.3 0.750 350 321 187 0.18 0.97 0.53AC2-HTT 90 0.648 14.5 0.700 83 63 66 0.05 0.78 0.28AC2-HTT-T 85 0.704 16.6 0.780 77 78 13 0.04 1.16 0.26AC3 14.5 275 0.566 4.1 0.610 269 274 100 0.19 1.13 0.40AC3-T 327 0.728 4.5 0.750 326 108 0.19 1.05 0.28AC3-HTT 108 0.545 10.1 0.630 100 70 11 0.08 1.15 0.12AC3-HTT-T 83 0.698 16.9 0.780 73 68 51 0.05 0.89 0.30GL 16.5 174 0.433 5.0 0.490 205 191 40 0.09 1.36 1.03GL-T 288 0.704 4.9 0.735 283 242 126 0.16 0.97 0.38GL-HTT 224 0.470 4.1 0.525 193 148 147 0.12 0.77 0.28GL-HTT-T 200 0.667 6.6 0.700 188 100 0.11 0.92 0.45
Z2 )n[1 + erf( xDS
θl(p,E) )Kp exp(zwΘ/kBT)
1 + Kp exp(zwΘ/kBT)(2)
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3149
equation of the first kind
where f(y) is the unknown distribution function of a givenparameter y (e.g., y ) E or Rp). A maximal p/p0 value for anisotherm portion used with eq 2 corresponds to nearly monolayercoverage. To calculate the f(y) functions with the overall isothermequation, a constrained regularization method can be used, asthe solution of eq 3 is a well-known ill-posed problem due to theimpact of noise on measured data, which does not allow one toutilize exact inversion formulas or iterative algorithms.16,17 Forthis purpose, the constrained regularization CONTIN procedure17
was modified to apply different local isotherm equations toestimate the distributions of the pore size and adsorption energy.
The pore size distribution was calculated by using the overallisotherm equation18
where rmin and rmax are the minimal and maximal half-width orthe pore radius, respectively; w ) 1 for slitlike pores and 2 forcylindrical pores;
b ) exp(∆ε/RgT); ∆ε is the excess of the evaporation heat due tothe interference of the layering on the opposite wall of pores;t(p,Rp) is the statistical thickness of adsorbed layer; am is theBET monolayer capacity; c ) cs exp((Qp - Qs)/RgT); cs is the BETcoefficient for adsorption on flat surface cs ) γe(E-QL/RgT), QL isthe liquefaction heat, E is the adsorption energy, and γ is aconstant; Qs and Qp are the adsorption heat on flat surface andin pores, respectively; z ) p/p0; n is the number (noninteger) ofstatistical monolayers of adsorbate molecules and its maximalvalue for a given Rp is equal to (Rp - σS/2)/tm; tm ) am/SBET; andσs is the collision diameter of surface atoms. Desorption data(total isotherms) were utilized to compute the f(Rp) distributionwith eq 4 and the regularization procedure under nonnegativitycondition with a fixed regularization parameter R ) 0.01.According to Nguyen and Do,18 eqs 4 and 6 are valid not only formesopores but also for micropores (in ref 18, xmin ) 0, butmicropores at the half-width xmin < 0.2 nm are inaccessible fornitrogen molecules, therefore one can assume xmin ) 0.2 nm ineq 4 that has not an influence on the positions of f(Rp) peaks).Several models of pores were applied for silica gel and carbosils,such as cylindrical pores for silica gel, slitlike pores at Rp < 2tmfor pyrocarbon, and pores as the gaps between sphericalpyrocarbon particles themselves and between these particles andsilica gel globules. In the last case, eq 5 should be replaced by10c
where R is the radius of pyrocarbon particles and t′ ) t + σs/2.Notice that the pore models have only a slight influence on thedistribution functions computed with eqs 3-7.
The f(Rp) distributions determined with eq 4 and linked todVp/dRp can be easily transformed to the distributions fS(Rp) withrespect to the derivative of the specific surface area dS/dRp using
the corresponding models of pores; e.g., for cylindrical pores
A similar regularization procedure for the overall isothermequation was usefully applied to compute the structural pa-rameters of pores of modified silica gels and carbons.19 Noticethat standard calculations of the pore size distributions (dVp/dRp or dS/dRp versus Rp) using the Barrett-Joyner-Halenda(BJH),20 deBoer,10,21 and Derjaguin-Broekhoff-deBoer-Dolli-more-Dubinin-Ulin13 equations gave incomplete pictures of thepore size distributions.7,8,19 At the same time, the regularizationprocedure CONTIN with eq 4 provides more detailed distributionfunctions f(Rp), which allow one to explore changes in micropores(Rp < 1 nm), mesopores (1 nm < Rp < 50 nm), and transportpores at Rp > 50 nm caused by different pretreatments of silicagels and carbosils. Additionally, the f(Rp) distributions computedwith eq 4 are close to those calculated with the DFT method,19g
but the last gave the distributions (for silica gels and carbons)close to those computed with eq 4, using only a portion of theisotherms at p/p0 > 0.01.
(d) NMR Investigation. The 1H NMR spectra were recordedusing a high-resolution WP-100 SY (Bruker) NMR spectrometerwith a bandwidth of 50 or 15 kHz. The isotropic value of thechemical shift of 1H (δH,iso) was referenced to tetramethylsilane(TMS). For water adsorbed on the silica surfaces from the gasphase, the chemical shifts were measured in CDCl3 media.Relative mean errors were (10% for signal intensity and (1 Kfor temperature. The technique of freezing-out of water wasapplied to separate bulk and interfacial waters in the aqueoussuspensions of silica gels or to distinguish different water layerson the adsorption from the gas phase.22-25 The amounts of theinterfacial unfrozen water (Cufw) in the aqueous suspensions ofsilica gels were estimated by comparison of an integral intensity(Iufw) of the 1H NMR signal of unfrozen water with that (Ic) ofwater adsorbed on oxide from the gas phase using a calibratedfunction Ic ) f(Cc), assuming Cufw ) (CcIufw/f(Cc)), or by comparisonof the water signals for liquid and gas phases at 285 K. Thesignals of surface hydroxyls and water molecules from ice werenot detected due to features of the measurement technique andthe short time (∼10-6 s) of cross-relaxation of protons in solids.
The free surface energy (γS in mJ/m2) was calculated (withrelative mean error (15%) using the known dependence ofchanges in the Gibbs free energy of ice on temperature
One can assume that water is frozen (T < 273 K) at the interfaceswhen G ) Gi and the value of ∆G ) G0 - G equals to ∆Gi )Gi|T)273K - Gi(T) and corresponds to a decrease in the Gibbs freeenergy of the interfacial water due to its interaction with thesolid surfaces (G0 denotes the Gibbs free energy of the bulkundisturbed water and ∆G > 0; i.e., the Gibbs free energy of the
(16) Szombathely, M.v.; Brauer, P.; Jaroniec, M. J. Comput. Chem.1992, 13, 17.
(17) Provencher, S. W. Comput. Phys. Commun. 1982, 27, 213; 229.(18) (a) Nguyen, C.; Do, D. D. Langmuir 1999, 15, 3608. (b) Nguyen,
C.; Do, D. D. Langmuir 2000, 16, 7218.
(19) (a) Gun’ko, V. M.; Leboda, R.; Zarko, V. I.; Marciniak, M.;Chibowski, E. Colloid. Surf. A, submitted for publication. (b) Gun’ko,V. M.; Leboda, R.; Skubiszewska-Zieba, J.; Rynkowski, J. J. ColloidInterface Sci. 2000, 231, 13. (c) Gun’ko, V. M.; Leboda, R.; Grzegorczyk,W.; Scubiszewska-Zieba, J.; Marciniak, M.; Malygin, A. A.; Malkov, A.A. Langmuir 2000, 16, 3227. (d) Gun’ko, V. M.; Leboda, R.; Charmas,B.; Villieras, F. Colloid Surf. A 2000, 173, 159. (e) Leboda, R.; Gun’ko,V. M.; Marciniak, M.; Malygin, A. A.; Malkin, A. A.; Grzegorczyk, W.;Trznadel, B. J.; Pakhlov, E. M.; Voronin, E. F. J. Colloid Interface Sci.1999, 218, 23. (f) Gun’ko, V. M.; Villieras, F.; Leboda, R.; Marciniak,M.; Charmas, B.; Skubiszewska-Zieba, J. J. Colloid Interface Sci. 2000,230, 320. (g) Gun’ko, V. M.; Do, D. D. Colloids Surf. A, in press.
(20) Barrett, E. P.; Joyner, L. G.; Halenda, P. P. J. Am. Chem. Soc.1951, 73, 373.
(21) Toth, J. Adv. Colloid Interface Sci. 1995, 55, 1.(22) Gun’ko, V. M.; Turov, V. V. Langmuir 1999, 15, 6405.(23) Gun’ko, V. M.; Zarko, V. I.; Turov, V. V.; Leboda, R.; Chibowski,
E. Langmuir 1999, 15, 5694.(24) Turov, V. V.; Leboda, R. Adv. Colloid Interface Sci. 1999, 79,
173.(25) Leboda, R.; Turov, V. V.; Marcyniak, M.; Malygin, A. A.; Malkov,
A. A. Langmuir 1999, 15, 8441.
Θ(T, p) ) ∫o
ymaxΘl(T, p, y) f(y) dy (3)
a ) ∫rmin
rk(p)f(Rp) dRp + ∫rk(p)
t(p, Rp)f(Rp) dRp (4)
2+ t(p,Rp) +
wγνm cos θ
[1 + (nb/2 - n/2)zn-1 - (nb + 1)zn + (nb/2 + n/2)zn+1]
[1 + (c - 1)z + (cb/2 - c/2)zn - (cb/2 + c/2)zn+1](6)
x(R + t′ + r)2 - R2 - r + R + t′] (7)
fs(Rp) ) 2Rp
∆Gi ) 0.036(273 - Γ) (9)
3150 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
interfacial water is lower than that of the bulk water). On thebasis of this approach, one can estimate the concentrations ofstrongly (Cs
ufw) and weakly (Cwufw) bound unfrozen waters, a
maximal reduction of the Gibbs free energy of strongly and weaklybound waters (∆Gs and ∆Gw), and free surface energy of adsorbentin aqueous medium (γS)
where K is a constant and Cmaxufw is the total amount of unfrozen
water at T f 273 K. The ∆G value in eq 10 is the differentialGibbs free energy, which is equal to the differential work ofadhesion
Therefore γS equals the total work of adhesion related to theinterface between the oxide and liquid phases. The force ofadhesion (per meter squared of the oxide surface) can becalculated by a simple equation
where X is the distance from the surface. For cylindrical poresin silica gels, X can be estimated as follows
assuming that the specific density of water in pores (Fufw) is equalto ≈1 g/cm3 and for a flat surface (or large pores)
Results and DiscussionThe Si-60 surface seems rough and granular and
globules forming large particles (0.1-0.2 mm) of silica gelare observed (Figure 1a) as well as large transport pores(dark areas in micrographs); however, main mesopores ofSi-60 at Rp < 10 nm are invisible due to relatively lowTEM magnification (24 000). After heating at 500 °C for
24 h in air, the silica gel surface appears slightly smoother,and granular structure is less visible (Figure 1b); however,significant changes in the pore characteristics do not occur(Table 1). After hydrothermal treatment (HTT) of Si-60at 150 °C for 6 h, the silica surface becomes spongy (Figure1c) and the specific surface area of both mesopores andmicropores significantly decreases; however, Vp is nearlythe same. After HTT at 200 °C, the spongy character ofthe surface becomes more clearly visible (Figure 1d), andVp and SBET (as well as Smes, SDS, etc.) decrease stronglydue to enlargement of pores and reduction of their numberbecause of disruption of the pore walls on the intensivehydrolysis of Si-O-Si bonds.26
Pyrocarbon grafting on the silica gel surfaces results information of both relatively large and practically nonpo-rous carbon particles (Figure 2a,b) and a carbon layerwith smaller graphene particles on the silica surfaces(Figure 2c). Both processes lead to reduction of the porosityand the specific surface area (as well as the accessibilityof pores blocked by carbon deposits) due to pore filling bypyrocarbon (Table 1), as the last formed from precursorsof small molecular sizes (under the used pyrolysis condi-tions) possesses low porosity (close to that of carbonblack).19,27 Additionally, the oxide matrix can be changedduring the pyrolysis due to chemical reactions withprecursor molecules or pyrolysis products (especially watermolecules formed from oxygen-containing reactants). Forexample, the glucose carbonization is accompanied by thelargest changes in the pore structure among preparedcarbosils (Table 1, GL). Notice that pyrocarbon includesnotonlypuregraphenestructuresbutalsooxidized groups,such as CdO, COH, C-O-C, and COOH, which canimpact the adsorptive properties of carbosils as the wholeor their particle characteristics in the aqueous suspen-sions.19,27
(26) Kiselev, A. V.; Lygin, V. I. IR Spectra of Surface Compounds andAdsorbed Substances, Nauka: Moscow, 1972.
(27) Gun’ko, V. M.; Skubiszewska-Zieba, J.; Leboda, R.; Zarko, V. I.Langmuir 2000, 16, 374.
Figure 1. TEM micrographs of (a) Si-60, (b) Si-60-T, (c) Si-60-HTT at THTT ) 150 °C, and (d) Si-60-HTT at THTT ) 200 °C.
γS ) K∫0
Cmaxufw∆G dCufw (10)
∆G ) -Wa (11)
F ) ∆G/X (12)
X ) Rp[1 - (1 -Cufw
X ) 3Cufw/S (14)
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3151
Hydrothermal treatment (HTT) of carbosils alters thepore parameters depending on CC (Table 1), due toshielding of the oxide surfaces by pyrocarbon depositsinhibiting hydrolysis of the silica pore walls (Figure 3a).However, marked differences in the surface structure incomparison with that of Si-60-HTT are not observed, e.g.,for AC3-HTT and AN2-HTT (Figure 1c and 3b,c). Similarresults are found for samples after HTT and subsequentheating at 500 °C in air (HTT-T) (Figure 4) depending onthe HTT temperature (THTT), which was higher for ACisamples. Thus, shielding of the oxide matrix by pyrocarbon
is responsible for smaller reduction of the specific surfacearea on HTT and HTT-T in comparison with that forSi-60-HTT and Si-60-HTT-T (Table 1).
The carbosil surfaces after heating at 500 °C for 24 h(Figure 4) are akin to those of Si-60-T (Figure 1b); however,S and V (Table 1) are smaller for carbosils than forSi-60-T due to chemical transformations of the pore wallsduring pyrolysis, especially for glucose containing largenumber of hydroxyls (which lead to the hydrolysis ofSi-O-Si bonds in the pore walls). On the other words,glucose carbonization is accompanied, in fact, by HTT of
Figure 2. TEM micrographs for (a) AC3, (b) GL, and (c) AN2.
Figure 3. TEM micrographs for (a) GL-HTT, (b) AC3-HTT, and AN2-HTT
3152 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
silica gel and the GL-T surface seems close to that of Si-60-HTT.
The RS plots10 for silica gels and carbosils (Figure 5,reference adsorption corresponds to Si-100028) show
significant changes in the porosity due to differenttreatments of adsorbents. However, dramatic changes inthe pore type are observed only after HTT at 200 °C ofsilica gels (Figure 5b) or ACi-HTT (Figure 5c). In the last
Figure 4. TEM micrographs for (a) AN2-T and (b) GL-T.
Figure 5. (a) Nitrogen isotherms for Si-60, initial and modified, and the RS plots for (b) Si-60, Si-40, and Si-100 pristine and treated,(c) initial and treated Aci and GL, and (d) initial and treated ANi.
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3153
case, these changes are smaller due to shielding of thesurfaces by pyrocarbon. For other samples, substantialalterations in the pore volume or the specific surface area(Table 1) can be rather due to blocking of pores bypyrocarbon particles, as the porosity of the last is low andthe specific surface area of pyrocarbon per se is providedby the external surfaces of carbon particles. A visibledisplacement of the plateau adsorption toward larger RSvalues for some modified samples (Figure 5) is linked toenlargement of the size of mesopores (Table 1, Rp), whichare filled by nitrogen at higher p/p0 (Figure 5a). Allsamples based on Si-60 demonstrate a low microporosity,as an initial linear part of their RS plots does not have asteep increase and points toward the origin of thecoordinates (Figure 5). Additionally, the specific surfacearea (SR) magnitudes determined on the basis of thisportion of the RS plots are close to both SBET and Smes(Table 1), and the micropore volume estimated with theRS plots for all samples is less than 0.01 cm3/g. The VDSand SDS values (Table 1) could be overestimated, as theywere computed without correction of the isotherms onadsorption in mesopores. A steep increase in adsorptionat RS > 1 for many of the samples (Figure 5) is linked withsecondary filling of mesopores (capillary condensationcorresponding to hysteresis loops, Figure 5a).
Theporevolume andthespecific surfacearea of carbosilsdecrease with CC independently of the origin of thepyrocarbon (Figure 6, Table 1). However, the precursortype and variations in pyrolysis conditions (temperatureand time),19 as well as the initial pore structure of silicagels (e.g., Si-40 and Si-60), impact the pore characteristicsof carbosils (Figures 6 and 7). For example, the narrowerthe pores of the pristine silica gel, the larger the specificsurface area reduction under the same pyrolysis conditions(Figure 5b, Si-40, average Rp ≈ 1.5 nm and Si-60, Rp ≈4 nm). Additionally, the pyrolysis of organics havingoxygen atoms in molecules leads to a greater decrease inthe specific surface area due to hydrolysis of Si-O-Sibonds and disruption of the pore walls (Figure 5, AC andGL). Notice that heating of Si-60 causes diminution of thehalf-width and dispersion of narrow pores (Table 1, xDS,δDS); i.e., micropores become more uniform. HTT of Si-60(especially at 200 °C) not only enhances the mesoporesizes but also strongly disrupts micropores, as SDS andVDS decrease by several times (Table 1) and minimal VDSis observed for Si-60-HTT-T at THTT ) 200 °C among allthe studied samples; however, minimal SDS is for ACi-HTT at the same THTT. Changes in the pore structure asa whole due to different pretreatments of various carbosils(Table 1, Figures 5-7) can be elucidated in detailsanalyzing the pore size distributions computed using theoverall isotherm approximation with the regularizationprocedure.
The regularization procedure with eq 4 fits adsorption-desorption isotherms for all the samples in faithfulagreement with experimental ones over the total p/p0range, which lends support to the validity of eq 4 for bothmicropores and mesopores. Additionally, the pore sizedistributions f(Rp) of Si-60, Si-40, and Si-100 calculatedwith eq 4 and the regularization procedure (fixed regu-larization parameter R ) 0.01 and nonnegativity conditionfor f(Rp)) using desorption data are close to dVp/dRpobtained with the frequently used Barrett-Joyner-Halenda (BJH) method at Rp > 1 nm (Figure 7b). However,eq 4 allows one also to compute f(Rp) for micropores at Rp
< 1 nm, therefore subsequent calculations of f(Rp) andfS(Rp) were performed only with eq 4. Notice that f(Rp)computed with eq 4 using desorption data is between dVp/dRp(BJH) for adsorption and desorption, which is clearlyseen for Si-100 (Figure 8). For all the studied samplesbased on Si-60, the f(Rp) peaks for micropores are verynarrow (notice that the log scale is used in Figures 8 and9) and give a small contribution to the pore volume.
Heating of Si-60 at 500 °C (Si-60-T) results in slightnarrowing of the main f(Rp) peak at Rp between 2 and 7nm (Figure 9a). However, a small f(Rp) peak at Rp > 10nm shifts toward larger Rp due to changes in the sizes ofnanoscaled silica globules on heating and correspondingrearrangement of mesopores. HTT of Si-60 at 150 °Cresults in reduction of all f(Rp) peaks (Vp slightly decreases)and displacement of the main mesopore peak toward Rp> 10 nm (Figure 9a). HTT of Si-60 at 200 °C givessignificant broadening of the pore size distribution, andsubsequent heating of the last sample enhances thisbroadening (Figure 9b).
The origin and amounts of pyrocarbon impact the mainmesopore f(Rp) peak at Rp > 2 nm (Figure 9c). The greatestchanges in mesopores and micropores (Table 1, Figure 9c)are observed for GL samples due to factual HTT of silicagel on the carbonization of glucose, which is a source ofwater molecules hydrolyzing Si-O-Si bonds in the pore
(28) (a) Jaroniec, M.; Kruk, M.; Olivier J. P. Langmuir 1999, 15,5410. (b) Jaroniec, M.; Kruk, M.; Jaroniec, C. P.; Sayari, A. Adsorption1999, 5, 39-45.
Figure 6. Relative changes in (a) SBET and Vp for carbosilswith Si-60 and (b) SBET for carbosils with Si-60 and Si-40 coveredby pyrocarbon of different origin.
3154 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
walls. A similar effect is observed for ACi samples, butdisplacement of f(Rp) for mesopores toward larger Rp issmaller due to a lower number of oxygen atoms inacetylacetone in comparison with glucose. Minimal changesin mesopores are observed for ANi samples (aromaticC12H10 as a precursor); however, changes in f(Rp) formicropores of ACi and ANi depend on CC larger than thatfor mesopores (Table 1) due to alteration in pyrocarbondistribution in matrix pores and on outer surfaces of silicagel particles in the form of relatively large globules(Figures 2-4).
Heating of carbosils at 500 °C for 24 h in air gives f(Rp)different from that for Si-60-T (Figure 9f). Consequently,pyrolysis of various precursors under the same conditionsis accompanied by distinct changes in the matrix porestructure, which are reflected by incomplete resuming ofpores on oxidizing of carbon deposits in air at 500 °C,especially for GL-T (Figure 9f, Table 1).
Significant changes in the pore structure of adsorbentsare observed due to their hydrothermal treatment (Figure9d). An increase in THTT for Si-60 from 150 °C (main portionof mesopores at Rp between 7 and 25 nm) to 200 °C giveslarger pores up to 200 nm with a very broadeneddistribution. In the case of ANi samples, pore enlargementdue to HTT is less than that for ACi (Figure 9d) becauseof the differences not only inTHTT but also in the pyrocarbondeposit characteristics (one prepared with acetylacetoneor glucose can include a large number of oxidized groups
in contrast to pyrocarbon prepared by the carbonizationof pure aromatics without O atoms in the molecules) andmodified (hydrolyzed)oxideporewalls.Theseeffects reflectin the mesopore and micropore parameters of ANi-HTTand ACi-HTT samples (Table 1) showing larger changesin ACi samples; i.e., pyrocarbon in ANi and GL samplesshields the oxide surfaces on HTT at 150 °C strongly thanthat for ACi on HTT at 200 °C. It seems likely that HTTof ACi at higher temperature has larger effect than thedifference in the origin of pyrocarbons. Subsequent heatingof HTT-samples (HTT-T) results in smaller changes inthe pore structure; however, mesopores become narrower(Figure 9e), as well as for pristine silica gel (Figure 9a,Table 1). For ANi-HTT-T samples, an increase in SBETand Vp is observed, but for ACi-HTT-T, SBET decreases(Table 1).
The fS(Rp) distribution functions with respect to thespecific surface area (dS/dRp) show that main contributionto S is given by pores at Rp < 10 nm (Figure 10). It shouldbe noted that relative contribution of micropores to Sincreases for all the samples after HTT, especially at THTT) 200 °C, with parallel disruption of main mesopores atRp between 2 and 6 nm. For carbosils, maximal contribu-tion of micropores to S is observed for AN1 and AC1 atlow CC (Figure 10a).
Thus, the pore structure depends not only the pre-treatment techniques but also on the origin of pyrocarbon(i.e., precursor composition). The last impacts the nitrogen
Figure 7. Specific surface area of (a) micropores (SDS) andmesopores (Smes) and SBET for treated samples as functions ofthe initial amounts of pyrocarbon and (b) pore volume of initialcarbosils versus CC.
Figure 8. Pore size distributions for Si-60, Si-40, and Si-100computed with eq 4 and BJH method using adsorption (BJHa)and desorption (BJHd) data; f(Rp) for Si-60 and Si-40 modifiedby the pyrolysis of acenaphthene at close CC values are alsoshown.
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3155
adsorption energy distributions (Figure 11a) causedmainly by dispersion interaction (plus electrostatic con-tribution due to polarization of N2 molecules interactingwith polar oxide surfaces, e.g., silanols). For ANi and ACi,the f(E) peak between 10 and 12 kJ/mol (adsorption in
broad micropores or narrow mesopores) shifts towardhigher energy with CC and it is markedly low for pristinesilica gel due to changes in the micropore structure ofadsorbent, as pores between primary silica gel globulesand pores between graphene sheets possess different
Figure 9. Pore size distribution computed with eq 4 with the regularization procedure (R ) 0.01) for (a) initial Si-60, Si-60-T,Si-60-HTT, and Si-40HTT at THTT )150 °C; (b) Si-100-HTT, Si-60HTT at THTT )200 °C and then heated at 500 °C for 24 h; carbosils(c) initial, (d) after HTT, (e) after HTT-T, and (f) after heating at 500 °C for 24 h.
3156 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
structural and absorptive characteristics.10 Heating of Si-60 in air at 500 °C for 24 h results in small changes in f(E),as the nature of the silica surfaces and pore structure arenearly the same; however, the f(E) peak at 12 kJ/mol islarger due to a displacement of f(Rp) for Si-60-T towardsmaller Rp for micropores. The f(E) peak at ≈22 kJ/molis linked with adsorption in the narrowest micropores atlow p/p0, and it is not shown for all samples as its intensityis very low. The f(E) peak at ≈6 kJ/mol corresponds toadsorption in broad mesopores and can be linked withsecondary (volume) filling of these pores atp/p0 > 0.110,15,19
and, clearly, is practically independent of the nature ofthe surfaces. HTT and HTT-T give a small displacementof f(E) peaks toward lower energy (Figure 12) due toenlargement of a major portion of pores and removal ofcarbon deposits.
Some structural features of different hydrothermallytreated silica gels (Si-40, Si-60, Si-100) can be elucidatedby using the 1H NMR method with freezing-out of adsorbed
water at T < 273 K.22-25 Vertical portions of the ∆G(Cufw)graphs (Figure 13a) are observed for the aqueous suspen-sions of initial silica gels Si-40 and Si-60 in contrast tononporous adsorbents,24 initial Si-100 (Figure 13a), andall hydrothermally treated samples (Figure 13b) possess-ing larger pores. Appearance of this portion of ∆G(Cufw)is due to unfreezing of the interfacial water in narrowpores with lowering temperature until T correspondingto a maximal ∆G value for this plot portion. On the otherwords, lowering T over some interval is not accompaniedby water freezing, as this water is under strong action ofthe silica surfaces in narrow pores, when electrostaticfields of the opposite pore walls strongly overlap.10 Asimilar effect was observed previously for water adsorbedon microporous carbons,24,29 whose ∆G(Cufw) plots are akinto that for initial Si-40.
(29) Leboda, R.; Turov, V. V.; Tomaszewski, W.; Gun’ko, V. M.;Skubiszewska-Zieba, J. Carbon, in press.
Figure 10. Pore size distribution with respect to dS/dRp for (a) initial Si-60 and carbosils, (b) Si-60 and ACi after HTT, (c) GLand ANi after HTT, and (d) Si-60 after HTT and HTT-T at THTT ) 200 °C.
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3157
The concentration of strongly bound water Csufw de-
creases with increasing pore size for both initial andhydrothermally treated silica gels (Table 2). The concen-tration of weakly bound water Cw
ufw is larger for the HTTsamples due to the enhancement of the pore size; however,the relationships between the Cw
ufw values for differentsilica gels (initial and HTT) are more complex than thosefor Cs
ufw (Table 2). Notice that the volume of unfrozenwater for HTT-200 samples is larger than their porevolume, maybe due to formation of thick water layers onthe outer surfaces of treated samples. Also, filling of largepores by nitrogen could be incomplete at p/p0 ≈ 0.98(estimation of Vp was made for this p/p0), in contrast tofilling by water in the aqueous suspensions.
The free surface energy γS is maximal for Si-60, initialor HTT. There can be several reasons for this result, asthe free surface energy at the silica/water interfacesdepends on both the nature (e.g., concentration of silanols,charge density) and the topography of the surfaces. HTTfor all samples leads to an increase in γS but by differentmagnitudes, and ∆γS (changes in γS due to HTT) ismaximally (236 mJ/m2) for Si-100HTT (Table 2). Ad-
ditionally, HTT results in a marked enhancement of ∆Gs,which characterizes the free energy of the first monolayerof adsorbed water. This value for HTT samples issignificantly greater than that for other materials inves-tigated previously,24,30 which can be due to a substantialincrease in the concentration of silanols (tSi-O-Sit +H2O f tSiOH + HOSit) (concentration of silanols fordifferent silicas in air can alter by several times7), capableof forming strong hydrogen bonds with water moleculesfrom the first layer with a larger number of such bondsper a molecule; i.e., the number of strongly bound watermolecules in the first layer increases for HTT samples.This circumstance leads to unusual behavior of the δH(T)functions for the HTT samples, as the average chemicalshift decreases with increasing water concentration at agiven temperature (Figure 14). However, for initial silicagels, the opposite result is observed. Notice that the F(X)function correlates with increasing pore size for HTT
(30) Gun’ko, V. M.; Zarko, V. I.; Turov, V. V.; Leboda, R.; Chibowski,E.; Pachlov, E. M.; Goncharuk, E. V.; Marciniak, M.; Voronin, E. F.;Chuiko, A. A. J. Colloid Interface Sci. 1999, 220, 302.
Figure 11. Nitrogen adsorption energy distribution calculatedusing eq 2 with the regularization procedure (R ) 0.01) for (a)initial silica and carbosils and (b) after heating at 500 °C for24 h.
Figure 12. Nitrogen adsorption energy distribution computedusing eq 2 with the regularization procedure (R ) 0.01) forsilica gel and carbosils after (a) HTT and (b) HTT-T; *150 °Cand **200 °C for Si-60.
3158 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
Figure 13. Changes in the Gibbs free energy of the interfacial water in the aqueous suspensions of initial (a) and hydrothermallytreated (b) Si-40, Si-60, and Si-100 and corresponding adhesion forces (c, d) and derivatives d(∆G)/dCufw as function of the distanceX (in Å) from the silica surface.
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3159
samples (Figure 13d), but such a correlation is absent forinitial silica gels (Figure 13c). A similar effect is seen forthe derivatives -d(∆G)/dCufw versus X (Figure 13e,f). The-d(∆G)/dCufw value is the analogue of the chemicalpotential for isobaric freezing of water. Maxima of thedependence of -d(∆G)/dCufw on X correspond to thedistances from the silica surfaces characterized morestable complexes (clusters) of the interfacial water. Theposition of these maxima shifts toward larger X with
increasing pore size for both initial and HTT silicas (HTTsamples, the X values were computed from a model of aflat surface). These effects can be explained by thesignificant differences in the unfrozen water layersdependent on the pore size. It should be noted that forSi-40, the -d(∆G)/dCufw maximum corresponds to a watermonolayer, but for Si-60 and Si-40HTT, this is three tofour monolayers, and for Si-60-HTT and Si-100-HTT, itis five to six water monolayers (Figure 13).
The δH(T) functions (Figure 14) were determined at theadsorbed water concentrations of 30-130 mg per gram ofsilica gels. These dependences do not have a simple shapein comparison with that for pure water (however, the lasthas a maximum at approximately 4.5 °C when the waterdensity is maximal; i.e., the hydrogen bond lengths areminimal resulting in larger δH
22) and differ significantlyfor initial and HTT samples. An incline for some portionsof the δH(T) plots is larger or smaller than that for purewater; i.e., the structure of the hydrogen bond network inthe interfacial water undergoes significant changes (de-
Figure 14. Chemical shift of 1H in the NMR spectra of water adsorbed from the gas phase as a function of the temperature atdifferent water concentrations on initial and hydrothermally (200 °C) treated Si-40 (a), Si-60 (b), and Si-100 (c); δH(T) is shownfor pure water.
Table 2. Parameters of the Bound Water Layer forAqueous Suspensions of Silica Gels, Initial and after
HTT at 200 °C
Si-40 3.2 570 92Si-60 3.5 1.5 540 210 172Si-100 3.25 0.8 500 250 87S-40HTT 5.0 0.7 300 320 281Si-60HTT 4.0 0.8 200 250 344Si-100HTT 4.0 0.75 180 270 323
3160 Langmuir, Vol. 17, No. 11, 2001 Gun’ko et al.
pending on the sample origin) due to interaction with thesilica surfaces. The number of hydrogen bonds peradsorbed molecule is less for Si-40, Si-40-HTT, and Si-60than that for pure water, Si-60-HTT, and Si-100. However,for Si-100-HTT, there are features in the δH(T) shapedependent on CH2O (Figure 14c) (or Cufw at T < 273 K,however, the CH2O values were chosen on the δH(T)measurements to provide Cufw ≈ CH2O over nearly the totaltemperature range). The δH value for a water moleculealone in CDCl3 is δH,0 ≈ 1.7 ppm, and for a molecule withfour hydrogen bonds in ice, δH,4 ≈ 7 ppm.31,32 The averagenumber (m) of the hydrogen bonds per molecule can beestimated as follows
The molecular mobility decreases with lowering temper-ature, which leads to the enhancement of the lifetime ofthe hydrogen bonds and a decrease in the intermolecularbond lengths, resulting in an increase in δH and m.Horizontal portions of the δH(T) plots can be caused byinsignificant changes in the structure of the interfacialwater with lowering temperature, e.g., in the m values.
ConclusionPyrocarbon forms relatively large globules on the
external surfaces of silica gel particles and covers the oxide
surfaces by tiny graphene particles. The largest structuralchanges are observed for adsorbents hydrothermallytreated at 200 °C.
The availability of oxygen atoms in pyrolyzed precursors(glucose, acetylacetone) has a substantial influence onthe structural parameters of carbosils (both pyrocarbonand silica) in comparison with those for carbosils preparedby acenaphthene carbonization. The temperature ofhydrothermal treatment and the origin of pyrocarbonimpact the pore structure, and the carbon deposit shieldingresults in smaller reduction of the specific surface area onsuch a treatment. Appearance of pyrocarbon on silica gelsurfaces influences the nitrogen adsorption energy dis-tributions mainly over the 9-15 kJ/mol range linked withadsorption in relatively narrow mesopores or broadmicropores, which markedly change during pyrolysis oforganics or subsequent hydrothermal or thermal treat-ments.
1H NMR investigations with freezing-out of the bulkwater in the aqueous suspensions of the initial andhydrothermally treated Si-60, Si-40, and Si-100 demon-strated changes in the structure of the interfacial waterfor HTT samples appearing in the corresponding depend-ences of the Gibbs free energy and chemical 1H shifts onadsorbed water concentration, temperature, and thesample origin.
Acknowledgment. This research was supported byNATO (Grant EST.CLG.976890) and the Polish StateCommittee for Scientific Research and Ministry of HighEducation and Science of Ukraine (Grant 2M/303-99).V.M.G. thanks Dr. S. W. Provencher for the CONTINprogram package.
(31) Gordon, A. J.; Ford, R. A. The Chemist’s Companion; Wiley:New York, 1972.
(32) Kinney, D. R.; Chuang, I. S.; Maciel, G. E. J. Am. Chem. Soc.1993, 115, 6786.
m )δH,obs - δH,0
Structure of Treated Silica Gel Langmuir, Vol. 17, No. 11, 2001 3161